Following the discovery of high-field superconductivity in the 1950, superconducting wires for magnet construction were produced in industry and offered for sale within a remarkably short space of time. By 1961 small magnets were being made from ¼ mm diameter wires of niobium zirconium, a ductile alloy. This was quickly followed by niobium tin, an intermetallic compound with excellent superconducting properties but so brittle that it could not be fabricated by conventional wire-drawing processes. It was initially produced for sale in the form of a vapour-deposited layer on a very thin stainless steel tape. Niobium titanium wires were first manufactured in 1965 and this ductile alloy has since become the standard
“work horse” of superconducting magnet construction, mainly because it is relatively easy to fabricate and can be co-processed with copper.
In this chapter we describe the fabrication of the two common technological
superconductors NbTi and Nb3Sn. In particular the Nb3Sn superconducting wires that
we have tested are made with the Modified Jelly Roll process (MJR), the Powder-in-
Tube process (PIT), and the Restacked Rod Process (RRP), which are described in the
4.2 Superconductors for use in magnets
An important issue for the development of new superconducting materials is to reach higher operating temperatures in order to reduce the cost of the cooling system.
However, at present only low temperature superconductors (LTS), operating at boiling helium temperature, are used to design and produce magnets, because the main demand on high current densities limits the choice of the material to be used.
The new high temperature superconductors (HTS) still do not reach very high current densities and are difficult to produce in the form of long thin wires .
The same request excludes using type I superconductors, where in the Meissner state current can flow only in a small part of the strand cross-section (delimited by the λ length) near the boundaries. Furthermore, these materials show a very low critical field, which limits applications. Hard type II superconductors are the only materials usable to manufacture magnets.
Over the last twenty years, niobium titanium alloys have undergone extensive development. Niobium titanium alloys are ductile and can be co-processed with copper into a wide range of composite conductors. NbTi is currently the most commonly used material in magnet industry, but its properties are adequate only up to fields of 8-9 T . MRI solenoids and superconducting accelerators, starting from the Tevatron, HERA, and more recently LHC have relied on NbTi. In addition, the Superconducting Super Collider (SSC), a U.S. project that was first approved and later cancelled, planned to use NbTi. Significant advances in performance as well as conductor cost reduction resulted from the SSC R&D.
For optimum performance, the critical parameters Jc
, and Tc
, should be as large as possible. In general, it turns out that critical field and temperature are determined by the chemistry of the material, like the composition, whereas the critical current density is determined by the microstructure .
Therefore, the Jc
of niobium titanium has increased as the processing techniques have been
Fig. 4.1 Critical current densities of NbTi and Nb3Sn at a constant
improved, whereas the critical field and temperature have remained more or less constant.
Fig. 4.1 shows the available operating area for a superconducting magnet using NbTi strands and Nb3
Sn strands. Nb3
Sn, which is an intermetallic compound with the A15 crystal structure, has an advantage over NbTi, both in terms of critical current density and critical field. In addition the critical temperature is appreciably higher for Nb3
Sn (18.3K) than for NbTi (9.3K). Despite these substantial advantages Nb3
Sn has been used so far only on a fairly modest scale in comparison with NbTi. The reason for this lies entirely in the mechanical properties of Nb3
Sn. Unlike NbTi, which is a ductile alloy, Nb3
Sn is a brittle intermetallic compound which critical current is extremely sensitive to tensile strains.
However, only A15 (Nb3
Sn and Nb3
Al) and HTS (Bi-2223, Bi-2212, and YBCO) materials could in principle be used above 10 T. As mentioned, HTS’s are not competitive yet. On short-term magnet production, Nb3
Sn appears to be the right choice, while Nb3
Al is the most promising on the medium term, showing less strain sensitivity.
4.2.1 Filamentary composites
The conductor used in magnet industry is not pure superconducting material.
Thin filaments of NbTi or Nb3
Sn are embedded in a copper matrix to form a multifilamentary strand. The need of implementing copper in the strand design was
Fig. 4.2 Nb3Sn multifilamentary strand.
described in section 3.3. The filaments have to be limited in size for two reasons, one of which is flux jumping, as explained in section 3.4.
The second reason to require small filaments is to limit persistent magnetization currents in the superconductor , which are the sources of severe field distortions at low excitation of an accelerator magnet. These bipolar currents generate all the multipoles allowed by the coil symmetry. A distinct hysteresis behavior is also observed. Actually the restriction on filament diameter is more constraining for magnetization than for flux jumping. For NbTi, filament diameters of 5-6 µm are needed for relative deviations from ideal dipoles or quadrupoles on the order of 10-
The filaments in a strand are also twisted with a pitch of 15-25 mm (more tightly than needed for stability against flux jumping) to suppress inter filament eddy currents induced during a field sweep across the matrix. Figure 3.2 shows a typical cross section for an Intermagnetics General Corp. (IGC) intermediate tin Nb3
Sn strand with 61 split-subelements before thermal reaction. The non-copper region containing the split-subelements is separated from the outer copper matrix by means of a tantalum barrier. Each subelement contains 106 Nb filaments.
4.3 Niobium Titanium
Niobium and titanium are mutually soluble to form ductile alloys over a wide range of compositions. The critical properties vary with composition. Since optimum critical field and highest critical temperature do not occur at the same composition, commercial alloys are usually formulated for optimum critical field, in the range of Nb 46.5 to 50 wt% Ti. Otherwise a compromise must be found depending on the technological application of the strand. A ternary element, most commonly tantalum, may also be added to produce a modest increase in Bc2
of 0.3 T at 4.2 K and 1.3 T at 1.8 K.
Originally it was thought that the principal source of flux pinning in the material
came from the dislocation cell structure in the wire. It has now become clear that most
of the pinning is provided by finely divided deposits of Ti α-phase. This is a
hexagonal close packed titanium rich phase, which is precipitated on the dislocation
cell boundaries as a result of the heat treatments applied during the manufacturing
process. The α phase remains normally resistive at low temperature and has been shown to be a significant source of flux pinning sites.
Artificial pinning center (APC) techniques have been attempted in order to increase the field operating range and critical current. These techniques are based on the fine dispersion of second phase particles by mechanical processing. So far they have only allowed achieving higher critical currents at low fields.
The request for higher field magnets has led to NbTi being used at temperatures lower than 4.2 K. This is the case of the Large Hadron Collider (LHC) at CERN. The magnets for this accelerator will work in superfluid helium (1.9K), where Bc2
is increased from its 4.2 K value of 11 T to 14 T. The use of superfluid helium brings many other benefits in terms of better cooling and stability.
The manufacturing technology has been developed by different firms.
Currently, the production of high Jc
wires with filaments below 10 µm embedded in a high purity OFHC (Oxygen Free High Conductivity) copper matrix is normal practice. A scheme is shown in Fig. 4.3.
Fig. 4.3 Production process of NbTi strands and cables.
The first step of the process is to build a billet of high homogeneity NbTi alloy by arc vacuum melting. The NbTi is then fitted inside a copper extrusion can with a thin diffusion barrier of pure Nb interposed between the NbTi and the copper. The purpose of this barrier is to prevent the formation of CuTi2
intermetallics during intermediate heat treatments, since they are hard and brittle, and break the filaments at the last stages of drawing. The billet is evacuated, electron-beam welded, and
Hexagonal rods steck and extrusion NbTi billet
assembly and extrusion
Cold drawing Drawing and twisting Cabling
extruded. After cold drawing to size, the rod is drawn through a hexagonal die and then cut into many lengths. These lengths are stacked into another copper can, which is again sealed, extruded and drawn down to final size. For accelerator magnets, which may have up to 104
filaments, a double stack process is often used in which the rods are again drawn into hexagonal sections and stacked in another can. Multiple heat treatments are applied throughout the process in a defined sequence of alternating cold work and heat treatment, which has been found to produce the best configuration of α Ti precipitates and hence the best flux pinning. After reaching final size, the wire is twisted.
Typical properties of NbTi strand produced for LHC dipoles are listed in Table 4.1.
4.4 Niobium Tin
Sn is an intermetallic compound having a well-defined stoichiometry and the A15 crystal structure . It shows higher critical temperature and field than NbTi, but is highly brittle, as previously mentioned, and its critical current is extremely strain sensitive. Originally, Nb3
Sn was produced in the form of tape by heating Nb tapes in a liquid Tin bath at temperatures above 930°C. However tapes are not a useful shape for magnet design, and new processing techniques had to be developed.
The basic elements Nb, Sn, and Cu are manufactured in the form of a round composite strand. At this stage, the strand is still ductile and can be used to produce cables.
The A15 compound is formed at the interface of Nb and the Cu-Sn matrix by heat treating such composites at temperatures of about 700°C. The Cu matrix is
Wire diameter [mm] 1.29
Filament diameter [µm] 5
Cu to non-Cu ratio 1.8
at 8 T and 4.2K [A/mm2
Table 4.1 NbTi properties for LHC
necessary to shorten the heat treatment time, since Cu works as a catalytic agent for the preferential growth of Nb3
Sn phase at the expense of other non superconducting Nb-Sn phases. Prior to heat treating the strand at high temperature to form the Nb3
Sn compound, heat treatments at lower temperature are necessary to homogenize the Cu- Sn matrix.
The dominant source of flux pinning in Nb3
Sn appears to be the grain boundaries . In order to obtain high critical current densities it is therefore necessary to produce a fine-grained structure. This is in conflict with the long time necessary to obtain a consistent volume of superconductor. The optimum process is obtained by balancing these two issues and taking into account the material specific application.
The critical current density, Jc
, needs to be carefully defined. In NbTi one normally quotes the critical current density in the superconductor, JcNbTi
, and the critical current density on the whole strand cross section, Jcav
. These two current densities are related to each other as follows:
= λ (4.1)
where λ is the copper to superconductor ratio. For Nb3
Sn the distinction is complicated by the presence of the bronze between the filaments, generated from the diffusion of tin into the copper. Usually the critical current density is calculated in the non-copper part of the strand, which is comprehensive of both superconductor and bronze, while the overall average value, Jcav
, is still calculated on the whole strand cross section.
Different manufacturing processes have been tested and developed in the last years by different companies. The most important ones are:
Internal tin process (IT);
Modified jelly roll process (MJR);
Restacked Rod Process (RRP);
Powder in tube process (PIT).
Heat treatments are determined and suggested by the manufacturing companies for each type of strand. In principle, this is done by trying various heat treatment schedules, testing the resulting properties of the strand, and choosing the thermal cycle that achieves the best strand performance.
4.4.1 The bronze process
The bronze process, although almost twenty years old, is still that used most frequently for large production of Nb3
Sn where reproducibility and reliability are essential and cost of little significance .
The bronze process is very similar to the fabrication of NbTi wires. A rod of pure ductile Nb or Nb containing a small amount of Ta or Ti is assembled in a bronze matrix, extruded, and drawn to the final size. The tin content in the bronze matrix being limited to less than 13.5wt% (limit for a ductile bronze alloy), a large bronze matrix is required to provide sufficient tin to the niobium rods. The initial billet is made of hundreds of Nb rods and it is drawn into a hexagonal shaped element of intermediate size. The hexagonal rods are cut and reassembled in a second billet, which is extruded, annealed and drawn to the final wire size. Nb3
Sn wires are stabilized against flux jumping using OFHC copper. The copper has to be protected from the diffusion of the bronze-tin by a tantalum or niobium barrier. The niobium barrier is cheaper, but at low fields it is superconducting . This can cause field distortions, which can become intolerable in applications like particle accelerator magnets. In these cases a Tantalum barrier is preferred. The stabilizing copper can be incorporated internally with up to 27% of the wire cross section or externally with a copper part of 30-60%.
The bronze process requires frequent annealing steps because bronze work hardens rapidly. If precautions are not taken, these multiple anneals result in pre- reaction between the Sn in the bronze and the Nb, with formation of Nb3
Sn during fabrication .
4.4.2 The internal tin process
The Internal Tin (IT) process was introduced to overcome the main limit of the
bronze method, which is a limited tin content of 13.5wt% in the matrix. A higher
concentration of tin produces higher critical current densities in the Nb3
Sn layer .
The idea was to distribute local tin sources surrounded by Nb rods and located in a copper tube. The composite Cu tube containing several Nb rods around a central hole is first hot extruded, then filled with Sn and drawn into hexagonal subelements, which are shortened and reassembled into a new billet characterized by a stabilizing copper outer ring protected by a tantalum barrier. The billet is then drawn to the final wire size without intermediate annealing. Since this process does not involve intermediate anneals during wire fabrication, the billets are free from prereaction problems.
Factors like the amount of Nb, the amount of Sn, the filament size and the subelement number characterize the conductor properties .
Fig. 4.5 Internal Tin (IT) by Intermagnetic General Corporation (IGC).
Sn NbFig. 4.4 Internal Tin Process.
S ta b iliz e r tu b e
S u b e le m e n t b u n d le
W ire d r a w in g E x tru d e d
c o m p o s ite tu b e
T in ro d W ir e
d r a w in g
S u b e le m e n t
Table 4.2 IGC ITER strand parameters
This method suffers from “bridging” problems . Since the Nb filaments around the Sn rod within a subelement are close together, they join or “bridge” during reaction when their volume increases after the conversion of Nb into the more voluminous Nb3
Sn. This leads to a so-called effective filament diameter much larger than the filament itself with flux jumps and large magnetization. This problem could be solved by spacing the filaments more widely apart. However, this would lower the overall Jc
, thus invalidating one of the chief advantages of the process.
Fig. 3.5 shows an unreacted IT wire of 1 mm diameter by Intermagnetics General Corporation (IGC). Its properties are presented in Table 4.2.
Property IGC ITER
Wire diameter [mm] 1.000 ± 0.001
Filament diameter [µm] 5
Number of subelements 19
Sn pool diameter [µm] 50
Cu stabilizer [%] 58.7 ± .03 Sn at.% in the non-Cu 10.1 Nb at.% in the non-Cu 20.4 Ic
at 12 T and 4.2K [A] > 200 Jc
at 12 T and 4.2K [A/mm2
] > 700 RRR ( ρCu@300K
) > 300
4.4.3 The modified jelly roll
The Modified Jelly Roll (MJR) is a variant of the internal tin method pursued by Teledyne Wah Chang company in the US. It consists of two parallel sheets of niobium and copper rolled around a solid tin rod. In this way the niobium part in the non-copper area is increased to 35%. The roll is inserted in a copper tube to form a billet. During drawing the niobium cross section is reduced by ~750 times and shaped as a hexagonal rod.
A second billet is then assembled using the hexagonal rods, and drawn to the
final wire size. No annealing is required during the process. Protecting barriers have
to be inserted between the tin core and the niobium sheet, between the niobium and copper sheets, and before the external stabilizing copper. For this purpose tantalum, vanadium, and niobium are used. Fig. 4.6 illustrates the main steps of this process.
The same factors as in the IT method characterize the conductor properties .
Like the IT process, this technology also suffers from filament “bridging” .
Fig. 4.7 shows an unreacted MJR wire of 1 mm diameter by Oxford Superconducting Technology (OST). Its properties are presented in Table 4.3.
Fig. 4.6 Modified jelly roll.
Fig. 4.7 Modified Jelly Roll (MJR) by Oxford Superconducting Technology.
Table 4.3 OST MJR strand parameters
4.4.4 The restacked rod process and the hot extruded rod process
Due to the high performance of Nb3
Sn made by internal Tin process, it is an attractive material for many types of large magnet systems. However, each application has its own special requirements that require some customisation of the strand. Material made for High Energy Physic (HEP) accelerator applications now have 12 T, 4.2 K Jc values of 3000 A/mm2, but require further development to reduce low field flux jump instabilities. Strands for ITER central solenoid coils have modest critical current density requirements, but very low hysteresis losses are important.
OI-ST (Oxford Instruments-Superconducting Technology) is working on several approaches to reduce the effective filament diameter, including subdividing the sub-elements, and restacking a larger number of sub-elements in the final restack billet.
Most of the internal tin strand is now made using the Restacked Rod Process (RRP). This method uses Nb rod extrusion, and replaces the older MJR process route.
Both the performance and yield of RRP strand are greater than for MJR process, and therefore RRP is more amenable to large-scale manufacturing.
One approach OI-ST has taken to scale-up the internal tin production is the development of the Hot Extruded Rod Process (HER) .
Property OST MJR
Wire diameter [mm] 1.000 ± 0.001 Filament diameter [µm] < 110
Number of subelements 54
Sn pool diameter [µm] 45
Cu stabilizer [%] 48 ± 0.03
Sn at.% in the non-Cu 16
Nb at.% in the non-Cu 50
at 12 T and 4.2K [A] > 800
at 12 T and 4.2K [A/mm2
] > 1900
RRR ( ρCu@300K
) < 20
The main steps of the HER process are: compacted salt is used as placeholders for Sn during extrusion of large strand billets; after the extrusion, the salt is removed and replaced with Sn rods .
The HER process, where the extrusion is hot, has successfully been used to fabricate a distributed barrier strand having 19-subelements . Although the hot extrusion step gives good and enables the fabrication of large internal tin billets, the requirement of putting the Sn rods in after extrusion limits the number of sub- elements in the restack to approximately 37(i.e. the size of the salt holes that the Sn goes into has a practical lower limit). Strand made in this way has reached a Jc (12 T, 4.2 K) of 2500 A/mm2
OI-ST also have developed a new method for supplying Ti to dope the Nb3
Sn, by substituting some of the Nb filaments in the sub-element billet with readily- available Nb-47wt%Ti alloy.
OI-ST is also developing strand for ITER. Strand has been produced with a Jc (12 T, 4.2 K) > 1100 A/mm2
, losses < 1000 mJ/cm3
. This lower-loss material was made using Nb-47wt%Ti rods to supply the Ti dopant to the remaining pure Nb filaments, thus replacing Sn-Ti. Elimination of Sn-Ti is desirable for scale-up, yield, and performance of ITER wire.
Figure 4.8 Restacked Rod Process (RRP), by Oxford Instruments- Superconducting Technology (OI-ST).
4.4.5 The powder in tube process
The Powder in Tube (PIT) process was first developed by the Netherlands Research Foundation and is presently adopted by the Shape Metal Innovation Company (SMI) . The basic idea is to fill hollow Nb tubes with fine granulated Nb2
Sn powder and then place them into a Cu matrix. Compared to other methods, a large portion of the non-active bronze content can be replaced by superconductor elements or stabilizing Cu. The non-reacted part of the outer Nb tube acts as barrier between Cu and Nb3
Sn. The development of this technique has allowed producing long 36 and 192 filament strands. In laboratory, samples of 1332 filament strands were also obtained . The next step for large scale PIT strand will be the realization of a 492 filaments strand with an effective filament diameter of about only 20 µm.
Factors like the number of sub-elements, the quality of the powders and the presence of a ternary element characterize the conductor properties .
Fig. 4.9 shows an unreacted PIT wire of 1 mm diameter SMI. Its properties are presented in Table 4.4.
50 µµµµm Cu
Figure 4.9 Powder-in-Tube (PIT) by Shape Metal Innovation Company (SMI).